Paper Number: RRV03-0007
An ASAE Meeting Presentation
Biodegradable Polymers: Past, Present, and Future
M. Kolybaba1, L.G. Tabil 1, S. Panigrahi1, W.J. Crerar1, T. Powell1, B. Wang1
Department of Agricultural and Bioresource Engineering
University of Saskatchewan
57 Campus Drive, Saskatoon, SK, CANADA S7N 5A9
Written for presentation at the
2003 CSAE/ASAE Annual Intersectional Meeting
Sponsored by the Red River Section of ASAE
Quality Inn & Suites
301 3rd Avenue North
Fargo, North Dakota, USA
October 3-4, 2003
Abstract. In recent years, there has been a marked increase in interest in biodegradable materials
for use in packaging, agriculture, medicine, and other areas. In particular, biodegradable polymer
materials (known as biocomposites) are of interest. Polymers form the backbones of plastic
materials, and are continually being employed in an expanding range of areas. As a result, many
researchers are investing time into modifying traditional materials to make them more user-friendly,
and into designing novel polymer composites out of naturally occurring materials. A number of
biological materials may be incorporated into biodegradable polymer materials, with the most
common being starch and fiber extracted from various types of plants. The belief is that
biodegradable polymer materials will reduce the need for synthetic polymer production (thus reducing
pollution) at a low cost, thereby producing a positive effect both environmentally and economically.
This paper is intended to provide a brief outline of work that is under way in the area of
biodegradable polymer research and development, the scientific theory behind these materials,
areas in which this research is being applied, and future work that awaits.
Keywords. biopolymer, biodegradable, plastic, agricultural products, biomaterial, recycling, life cycle
assessment, environmental impact, economic impact, compost
The authors are solely responsible for the content of this technical presentation. The technical presentation does not necessarily
reflect the official position of the American Society of Agricultural Engineers (ASAE), and its printing and distribution does not
constitute an endorsement of views which may be expressed. Technical presentations are not subject to the formal peer review
process by ASAE editorial committees; therefore, they are not to be presented as refereed publications. Citation of this work should
state that it is from an ASAE meeting paper EXAMPLE: Author's Last Name, Initials. 2003. Title of Presentation. ASAE Paper No.
03xxxx. St. Joseph, Mich.: ASAE. For information about securing permission to reprint or reproduce a technical presentation, please
contact ASAE at email@example.com or 269-429-0300 (2950 Niles Road, St. Joseph, MI 49085-9659 USA).
The development of innovative biopolymer materials has been underway for a number of years,
and continues to be an area of interest for many scientists. In 1996, shipments from the
Canadian Plastic Industry increased by 10.6% from 1995 levels (Charron 1999), to $9.1 billion.
Fomin (2001) reported that the end of the 20th century saw the worldwide production of synthetic
plastics reach 130 million t/year, while the demand for biodegradable plastics is reported to be
growing by 30% each year (Leaversuch 2002). European countries have reported an estimated
average usage of 100kg of plastic per person each year (Mulder 1998).
Synthetic plastics are resistant to degradation, and consequently their disposal is fuelling an
international drive for the development of biodegradable polymers. As the development of
these materials continues, industry must find novel applications for them. Material usage and
final mode of biodegradation are dependent on the composition and processing method
employed. An integrated waste management system may be necessary in order to efficiently
use, recycle, and dispose of biopolymer materials (Subramanian 2000). Reduction in the
consumption of sources, reuse of existing materials, and recycling of discarded materials must
all be considered.
Polymer materials are solid, non-metallic compounds of high molecular weights. (Callister
2000). They are comprised of repeating macromolecules, and have varying characteristics
depending upon their composition. Each macromolecule that comprises a polymeric material is
known as a mer unit. A single mer is called a monomer, while repeating mer units are known as
polymers. A variety of materials (both renewable and non-renewable) are employed as
feedstock sources for modern plastic materials. Plastics that are formed from non-renewable
feedstocks are generally petroleum-based, and reinforced by glass or carbon fibers (Williams et
al. 2000). Renewable resource feedstocks include microbially-grown polymers and those
extracted from starch. It is possible to reinforce such materials with natural fibers, from plants
such as flax, jute, hemp, and other cellulose sources (Bismarck et al. 2002).
Economic concerns must be addressed objectively as biopolymer materials are developed,
because the future of each product is dependent on its cost competitiveness, and society’s
ability to pay for it. Many governments are introducing initiatives designed to encourage
research and development of biologically based polymers. Most European and North American
politicians and policy makers support work in this area, with the German government being
particularly interested (Grigat et al. 1998).
The future outlook for advancement in the area of biodegradable plastics is ultimately promising.
Canada’s biotechnology infrastructure is world class, with the provinces of Ontario, Quebec, and
Saskatchewan being particularly active and successful in research and development. Crawford
(2001) explained that Canada’s long term goal on the international front is to develop
technologies that are able to accept a diverse combination of raw materials, and produce
multiple outputs, while releasing no emissions.
This literature review is intended to provide information regarding progress made in the
development of biodegradable polymer materials. Biodegradability, constituent materials,
applications, methods of biodegradation and environmental and economic implications of such
materials will be examined. Finally, information regarding the future direction for biodegradable
polymers will be objectively discussed.
BIODEGRADABILITY OF POLYMERS
The American Society for Testing of Materials (ASTM) and the International Standards
Organization (ISO) define degradable plastics as those which undergo a significant change in
chemical structure under specific environmental conditions. These changes result in a loss of
physical and mechanical properties, as measured by standard methods. Biodegradable plastics
undergo degradation from the action of naturally occurring microorganisms such as bacteria,
fungi, and algae. Plastics may also be designated as photodegradable, oxidatively degradable,
hydrolytically degradable, or those which may be composted. Between October 1990 and June
1992, confusion as to the true definition of “biodegradable” led to lawsuits regarding misleading
and deceitful environmental advertising (Narayan et al. 1999). Thus, it became evident to the
ASTM and ISO that common test methods and protocols for degradable plastics were needed.
There are three primary classes of polymer materials which material scientists are currently
focusing on. These polymer materials are usually referred to in the general class of plastics by
consumers and industry. Their design is often that of a composite, where a polymer matrix
(plastic material) forms a dominant phase around a filler material (Canadian Patent #2350112-
2002). The filler is present in order to increase mechanical properties, and decrease material
Conventional plastics are resistant to biodegradation, as the surfaces in contact with the soil in
which they are disposed are characteristically smooth (Aminabhavi et al. 1990).
Microorganisms within the soil are unable to consume a portion of the plastic, which would, in
turn, cause a more rapid breakdown of the supporting matrix. This group of materials usually
has an impenetrable petroleum based matrix, which is reinforced with carbon or glass fibers.
The second class of polymer materials under consideration is partially degradable. They are
designed with the goal of more rapid degradation than that of conventional synthetic plastics.
Production of this class of materials typically includes surrounding naturally produced fibers with
a conventional (petroleum based) matrix. When disposed of, microorganisms are able to
consume the natural macromolecules within the plastic matrix. This leaves a weakened
material, with rough, open edges. Further degradation may then occur.
The final class of polymer materials is currently attracting a great deal of attention from
researchers and industry. These plastics are designed to be completely biodegradable. The
polymer matrix is derived from natural sources (such as starch or microbially grown polymers),
and the fiber reinforcements are produced from common crops such as flax or hemp.
Microorganisms are able to consume these materials in their entirety, eventually leaving carbon
dioxide and water as by-products.
Materials must meet specific criteria set out by the ASTM and ISO in order to be classified as
biodegradable. In general, the likelihood of microbial attack on a material is dependent on the
structure of the polymer. When examining polymer materials from a scientific standpoint, there
are certain ingredients that must be present in order for biodegradation to occur. Most
importantly, the active microorganisms (fungi, bacteria, actinomycetes, etc.) must be present in
the disposal site. The organism type determines the appropriate degradation temperature,
which usually falls between 20 to 60oC (Shetty et al. 1990). The disposal site must be in the
presence of oxygen, moisture, and mineral nutrients, while the site pH must be neutral or
slightly acidic (5 to 8).
Biodegradation of materials occurs in various steps (Aminabhavi et al. 1990). Initially, the
digestible macromolecules, which join to form a chain, experience a direct enzymatic scission.
This is followed by metabolism of the split portions, leading to a progressive enzymatic
dissimilation of the macromolecule from the chain ends. Oxidative cleavage of the
macromolecules may occur instead, leading to metabolization of the fragments. Either way,
eventually the chain fragments become short enough to be converted by microorganisms
Biodegradable polymers (those derived from plant sources) begin their lifecycle as renewable
resources, usually in the form of starch or cellulose. As reported by Lorcks (1998), innovative
polymer research and development leads to large scale production by plastic converters. The
biopolymers are formed into the specific end products and used by a consumer. Ideally, the
biopolymer will be disposed in a bio waste collection, and later composted. This process will
ultimately leave behind carbon dioxide and water, which are environmentally friendly by-
BIOLOGICAL MATERIALS AND BIODEGRADABLE PLASTICS
Naturally occurring biopolymers are derived from four broad feedstock areas (Tharanathan
2003). Animal sources provide collagen and gelatine, while marine sources provide chitin which
is processed into chitosan. However, the remaining two feedstock areas are the ones receiving
the most attention from scientists, and are the sources thought to be the most promising for
future development and expansion. Microbial biopolymer feedstocks are able to produce
polylactic acid (PLA) and polyhydroxy alkanoates (PHA). The final category of agricultural
feedstocks are the biopolymer source under consideration at the University of Saskatchewan, in
Saskatoon, Canada. This variety of polymers falls into the categories of hydrocolloids, and
lipids and fats.
Starch is an agricultural feedstock hydrocolloid biopolymer found in a variety of plants including
(but not limited to) wheat, corn, rice, beans, and potatoes (Salmoral et al. 2000, Martin et al.
2001). Starch is usually utilized in the form of granules, and is actually formed by one branched
and one linear polymer (Chandra et al. 1998). Amylose, the linear polymer, comprises
approximately 20% w/w of starch, while Amylopectin, the branched polymer, constitutes the
remainder. Natural filler materials may be incorporated into synthetic plastic matrices as a
rapidly biodegradable component. Often, granular starch is added to polyethylenes in order to
increase the degradation rate of the plastic material.
Starch can also be used in its gelatinized form (Verhooght et al. 1995). Heating the starch in
the presence of water during extrusion or injection moulding causes the formation of a
thermoplastic material that may be deformed during blending. This starch-based product is then
blended with either natural or synthetic materials. Heating starch above its glass transition
temperature breaks its molecular structure, allowing further bonding (Jopski 1993). Glycerol is
often used as a plasticizer in starch blends, to increase softness and pliability. Starch granules
that have been plasticized with water and glycerol are referred to as plasticized starches (Martin
et al. 2001). Plastic materials that are formed from starch-based blends may be injection
molded, extruded, blown, or compression molded.
Agricultural feedstocks for the biopolymer industry also include fibres that are used as
reinforcing fillers. This classification includes cellulose, which is the highly polar, main structural
component of flax and hemp fibres (Bismarck 2002). Natural cellulose fibres are low cost,
biodegradable, and have strong mechanical properties. These characteristics make cellulose
fibres the most common choice for natural fillers in plastic materials. Hornsby et al. (1997)
concluded that the presence of 25% w/w of cellulose fibres in a polypropylene matrix causes a
significant increase in tensile modulus. Cellulose has a very long molecular chain, which is
infusible and insoluble in all but the most aggressive solvents (Chandra et al. 1998). Therefore,
it is most often converted into derivatives to increase solubility, which further increases adhesion
within the matrix.
Canadian researchers are particularly interested in expanding the area of fiber use in
biopolymer products, as this would allow for value added processing of local agricultural waste
products. Flax fibres continue to receive the majority of the consideration, as they are
mechanically strong and readily available. Chemical treatment (acetylation) of the fibres is
performed in order to modify the surface properties, without changing the fiber structure and
morphology (Frisoni 2001). These modifications slow down the initiation of degradation of the
fibres, and increase adhesion at the fiber and matrix interface. Bledzki et al. (1999) concluded
that fibres that have been thoroughly dried prior to being added to the matrix show improved
adhesion as opposed to fibres with a higher moisture content. Research has shown that
polyvinyl alcohol is an appropriate polymer to use as a matrix in natural fiber reinforced
composites, as it is highly polar and biodegradable (Chiellini et al. 2001).
Microbial biopolymer feedstocks produce biological polymers through microbial fermentation.
The products are naturally degradable, environmentally friendly substitutes for synthetic plastics
(Chau et al. 1999). A number of bacteria accumulate polyhydroxy alkanoates (PHAs) as
intracellular carbon reserves when nutrient deficiencies occur. The biopolymers, which are
microbially produced polyesters, have the same thermoplastic and water resistant qualities as
synthetic plastics. It was concluded by Chau et al. (1999) that increasing the carbon to nitrogen
(C:N) ratio in a chemical wastewater treatment system increased specific polymer yield (ie, the
production of PHA’s increased). Researchers have long been aware that practically any type of
biomass can be converted into sugars through chemical or biological treatments. Certain
organisms are then capable of forming PHAs from the sugars. Such is the case at the
University of Hawaii, where food waste is being converted into PHAs (Petkewich 2003). Work in
these areas continues, as the issue constricting expansion in the development of industry-wide
PHA use is the high cost of producing the material. PHAs are brittle and expensive when used
alone, so researchers opt to blend them with less expensive polymers, which have
Polylactic acid is the second common biopolymer which is produced by microbial fermentation.
It is produced by the condensation of lactic acid, which is obtained through fermentation
processes (Jopski, 1993). Wilkinson Manufacturing Co. (Fort Calhoun, Nebraska, USA) has
recently introduced a commercially available thermoformed all-natural plastic container using a
corn-based PLA. The carbon stored in the plant starches is broken down to natural plant
sugars. Fermentation and separation form the PLA. PHA and PLA are both considered
synthetic polymers, as they are not found in nature. However, they are wholly biodegradable
There are a number of other biological materials that have been examined and manipulated by
biopolymer researchers. Wheat contains starch and gluten, both of which are employed by the
biopolymer industry. Canola derivatives have potential as both polymers and plasticizers
(Crawford 2001). Chitosan is obtained from the deacetylation of chitin, which is found in marine
environments. Because it is insoluble in water, chitosan is dissolved in acidic solutions before
being incorporated into biodegradable polymer films (Park et al. 2001). The structural
characteristics of soy proteins give them potential for industrial applications in plastics and
reinforced composite materials (Park et al. 2000). As a general conclusion, it can be stated that
many naturally occurring organisms (plant and animal) have potential to be modified and
employed as biopolymers.
APPLICATIONS FOR BIODEGRADABLE POLYMERS
Research and development is only a portion of the work that is done in order to introduce the
use of biodegradable polymer materials. The design of such materials usually begins with a
conceptual application. It may be expected to replace an existing material, or to complement
one. Sectors where applications for biopolymers have introduced include (but are not limited to)
medicine, packaging, agriculture, and the automotive industry. Many materials that have been
developed and commercialized are applied in more than one of these categories.
Biopolymers that may be employed in packaging continue to receive more attention than those
designated for any other application. All levels of government, particularly in China (Chau et al.
1996) and Germany (Bastioli 1998), are endorsing the widespread application of biodegradable
packaging materials in order to reduce the volume of inert materials currently being disposed of
in landfills, occupying scarce available space. It is estimated that 41% of plastics are used in
packaging, and that almost half of that volume is used to package food products.
BASF, a world leader in the chemical and plastic industry, is working on further development of
biodegradable plastics based upon polyester and starch (Fomin et al. 2001). Ecoflex is a fully
biodegradable plastic material that was introduced to consumers by BASF in 2001. The
material is resistant to water and grease, making it appropriate for use as a hygienic disposable
wrapping, fit to decompose in normal composting systems. Consequently, Ecoflex has found a
number of applications as a packaging wrap.
Environmental Polymers (Woolston, Warrington, UK) has also developed a biodegradable
plastic material. Known as Depart, the polyvinyl alcohol product is designed for extrusion,
injection molding, and blow molding. Depart features user-controlled solubility in water, which is
determined by the formulation employed. Dissolution occurs at a preset temperature, allowing
the use of Depart in a variety of applications. Examples include hospital laundry bags which are
“washed away” allowing sanitary laundering of soiled laundry, as well as applications as
disposable food service items, agricultural products, and catheter bags (Blanco 2002).
The renewable and biodegradable characteristics of biopolymers are what render them
appealing for innovative uses in packaging. The end use of such products varies widely. For
example, biodegradable plastic films may be employed as garbage bags, disposable cutlery and
plates, food packaging, and shipping materials. Guan and Hanna (2002) documented how
biodegradable loose-fill packaging materials may be developed from renewable biopolymers
such as starch. The starch material is treated by an acetylation process, chemical treatments,
and post-extrusion steaming. Mechanical properties of the material are adequate, and true
biodegradability is achieved.
The biopolymer materials suited for packaging are often used in agricultural products. Ecoflex,
in particular, sees use in both areas. Young plants which are particularly susceptible to frost
may be covered with a thin Ecoflex film. At the end of the growing season, the film can be
worked back into the soil, where it will be broken down by the appropriate microorganisms. Li et
al. (1999) concluded that the use of a clear plastic mulch cover immediately following seeding
increases the yield of spring wheat if used for less than 40 days. Therefore, plastic films that
begin to degrade in average soil conditions after approximately one month are ideal candidates
as crop mulches.
Agricultural applications for biopolymers are not limited to film covers. Containers such as
biodegradable plant pots and disposable composting containers and bags are areas of interest
(Huang 1990). The pots are seeded directly into the soil, and breakdown as the plant begins to
grow. Fertilizer and chemical storage bags which are biodegradable are also applications that
material scientists have examined. From an agricultural standpoint, biopolymers which are
compostable are important, as they may supplement the current nutrient cycle in the soils where
the remnants are added.
The medical world is constantly changing, and consequently the materials employed by it also
see recurrent adjustments. The biopolymers used in medical applications must be compatible
with the tissue they are found in, and may or may not be expected to break down after a given
time period. Mukhopadhyay (2002) reported that researchers working in tissue engineering are
attempting to develop organs from polymeric materials, which are fit for transplantation into
humans. The plastics would require injections with growth factors in order to encourage cell
and blood vessel growth in the new organ. Work completed in this area includes the
development of biopolymers with adhesion sites that act as cell hosts in giving shapes that
mimic different organs.
Not all biopolymer applications in the field of medicine are as involved as artificial organs. The
umbrella classification of bioactive materials includes all biopolymers used for medical
applications. One example is artificial bone material which adheres and integrates onto bone in
the human body. The most commonly employed substance in this area is called Bioglass
(Kokubo 2003). Another application for biopolymers is in controlled release delivery of
medications. The bioactive material releases medication at a rate determined by its enzymatic
degradation (Sakiyama-Elbert et al. 2001) PLA materials were developed for medical devices
such as resorbable screws, sutures, and pins (Selin 2002). These materials reduce the risk of
tissue reactions to the devices, shorten recovery times, and decrease the number of doctor
visits needed by patients.
The automotive sector is responding to societal and governmental demands for environmental
responsibility. Biobased cars are lighter, making them a more economical choice for
consumers, as fuel costs are reduced. Natural fibres are substituted for glass fibres as
reinforcement materials in plastic parts of automobiles and commercial vehicles (Lammers and
Kromer 2002). An additional advantage of using biodegradable polymer materials is that waste
products may be composted. Natural fibres (from flax or hemp) are usually applied in formed
interior parts. The components do not need load bearing capacities, but dimensional stability is
important. Research and development in this area continues to be enthusiastic, especially in
There are a number of novel applications for biopolymers, which do not fit into any of the
previous categories. One such example is the use of biopolymer systems to modify food
textures. For example, biopolymer starch (gelatin-based) fat replacers possess fat-like
characteristics of smooth, short plastic textures that remain highly viscous after melting.
Research continues into high pressure being used to manipulate biopolymers into food
products. The eventual goal is improved physical characteristics such as foaming, gelling, and
water- or fat-binding abilities (Ledward 1993). Biopolymer materials are currently incorporated
into adhesives, paints, engine lubricants, and construction materials (Fomin et al. 2001).
Biodegradable golf tees and fishing hooks (Canadian Patent # 2198680-1997) have also been
invented. The attraction of biopolymers in all of these areas is their derivation from renewable
sources, slowing the depletion of limited fossil fuel stores.
METHODS OF BIODEGRADATION
Just as important as the way in which a material is formed is the way in which it is degraded. A
general statement regarding the breakdown of polymer materials is that it may occur by
microbial action, photodegradation, or chemical degradation. All three methods are classified
under biodegradation, as the end products are stable and found in nature.
Many biopolymers are designed to be discarded in landfills, composts, or soil. The materials
will be broken down, provided that the required microorganisms are present. Normal soil
bacteria and water are generally all that is required, adding to the appeal of microbially reduced
plastics (Selin 2002). Polymers which are based on naturally grown materials (such as starch
or flax fiber) are susceptible to degradation by microorganisms. The material may or may not
decompose more rapidly under aerobic conditions, depending on the formulation used, and the
In the case of materials where starch is used as an additive to a conventional plastic matrix, the
polymer in contact with the soil and/or water is attacked by the microbes. The microbes digest
the starch, leaving behind a porous, spongelike structure with a high interfacial area, and low
structural strength. When the starch component has been depleted, the polymer matrix begins
to be degraded by an enzymatic attack. Each reaction results in the scission of a molecule,
slowly reducing the weight of the matrix until the entire material has been digested (Shetty et al.
Another approach to microbial degradation of biopolymers involves growing microorganisms for
the specific purpose of digesting polymer materials. This is a more intensive process that
ultimately costs more, and circumvents the use of renewable resources as biopolymer
feedstocks. The microorganisms under consideration are designed to target and breakdown
petroleum based plastics (Andreopoulos et al. 1994). Although this method reduces the volume
of waste, it does not aid in the preservation of non-renewable resources.
Photodegradable polymers undergo degradation from the action of sunlight (ASTM 883-96). In
many cases, polymers are attacked photochemically, and broken down to small pieces. Further
microbial degradation must then occur for true biodegradation to be achieved. Polyolefins (a
type of petroleum-based conventional plastic) are the polymers found to be most susceptible to
photodegradation. Proposed approaches for further developing photodegradable biopolymers
includes incorporating additives that accelerate photochemical reactions (e.g. benzophenone),
modifying the composition of the polymers to include more UV absorbing groups (e.g. carbonyl),
and synthesizing new polymers with light sensitive groups (Andreopoulos et al. 1994). An
application for biopolymers which experience both microbial and photodegradation is in the use
of disposable mulches and crop frost covers.
Some biodegradable polymer materials experience a rapid dissolution when exposed to
particular (chemically based) aqueous solutions. As mentioned earlier, Environmental
Polymer’s product Depart is soluble in hot water. Once the polymer dissolves, the remaining
solution consists of polyvinyl alcohol and glycerol. Similar to many photodegradable plastics,
full biodegradation of the aqueous solution occurs later, through microbial digestion. The
appropriate microorganisms are conveniently found in wastewater treatment plants (Blanco
2002). Procter & Gamble has developed a product similar to Depart, named Nodax PBHB.
Nodax is alkaline digestible, meaning that exposure to a solution with a high pH causes a rapid
structural breakdown of the material (Leaversuch 2002). Biopolymer materials which
disintegrate upon exposure to aqueous solutions are desirable for the disposal and transport of
biohazards and medical wastes. Industrial “washing machines” are designed to dissolve and
wash away the aqueous solutions for further microbial digestion.
ENVIRONMENTAL IMPACTS OF BIOPOLYMERS
Engineers are attempting to integrate environmental considerations directly into material
selection processes, in order to respond to an increased awareness of the need to protect the
environment (Thurston et al. 1994). The use of renewable resources in the production of
polymer materials achieves this in two ways. First of all, the feedstocks being employed can be
replaced, either through natural cycles or through intentional intervention by humans. The
second environmental advantage of using renewable feedstocks for biopolymer development is
the biodegradable nature of the end products, thereby preventing potential pollution from the
disposal of the equivalent volume of conventional plastics. At the end of their useful period,
biopolymer materials are generally sent to landfills or composted.
Recycling of plastic materials is encouraged and well advertised, but attempts at expanding this
effort have been less than effective. In the United States, currently less than 10% of plastic
products are recycled at the end of their useful life (Chiellini et al. 2001). Recycling must be
recognized as a disposal technique, not a final goal for material development. A complacent
attitude regarding recycling processes ignores the fact that advanced infrastructure is needed to
properly house recycling. As Mulder (1998) discovered, in underdeveloped countries plastics
are almost completely recycled, as the return on investment is positive in their economic
situation. This appears to be positive at the onset, but the open systems by which the plastics
are recycled allow the emission of toxic gases at crucial levels.
Recycling appeared to be a viable way to reduce pollution and environmental damage when it
was first introduced as a waste reduction technique. However, as time has passed, it is now
obvious that the use of plastics based on renewable feedstocks which are biodegraded is a
more sensible choice than recycling conventional plastics, as the end products are organic
matter, and toxic emissions are avoided. Therefore, growth of plastics which are compostable
or easily degraded must be encouraged.
In recent years, concern about a perceived garbage crisis has grown. Landfills have reached
capacity, and sites for new landfills are difficult to find. When biopolymers are disposed in
landfill environments, the hope is that the necessary microorganisms will be present. Unless
the soil is inoculated with them, this may not always be the case. As reported by Petkewich
(2003), carrots have been found to remain orange, and grass clippings green, after years in a
landfill. Inoculation with bacteria, fungi, and actinomycetes is effective in encouraging
biopolymer breakdown within soil (Orhan et al. 2000). However, if the appropriate
microorganisms are present, the disposal (and consequential breakdown) of biodegradable (or
partially biodegradable) plastic materials will lead to an increase of available space in current
landfills as the volume of waste is reduced through biodegradation (Simon et al. 1998).
Compostable plastics undergo biological degradation during composting to yield carbon dioxide,
water, inorganic compounds, and biomass at a rate consistent with other known compostable
materials, and leave no visually distinguishable or toxic residues (ASTM 1996). Many of the
biodegradable plastic materials discussed thus far were designed to be compostable. For
instance, the purpose of designing disposable plastic cutlery and plates is that they can be
thrown into a compost heap with leftover food. The requirements of biopolymers to be included
in industrial composters are complete biodegradation and disintegration, and that there be no
effect on compost quality as a result of biopolymer degradation (Wilde and Boelens 1998).
As an added benefit, Nakasaki et al. (2000) concluded that odor emissions from compost piles
are reduced when biodegradable plastic is included in the mix. Ammonia, a noxious gas, is
produced by the decomposition of compost. The degradation of biodegradable plastics
produces acidic intermediates, which neutralize the ammonia content, thus reducing odor
The 1970’s began an era of increased factual thinking processes by researchers and industry
officials. As such, the technique of life cycle analysis (LCA) emerged. This modeling exercise
is based on a simple idea; it is necessary to look at the complete life cycle for the production,
use, and disposal of a product in order to obtain a clear picture of the true environmental
implications of its development (Boustead 1998). Performing an LCA demonstrates whether or
not further development of a product is a viable option. There are three steps to an LCA,
beginning with the inventory, where inputs and outputs of the system are quantitatively
described. The interpretation step follows, which links the inputs and outputs with observable
environmental effects. Finally, the improvement step is carried out. Here, the system is
redesigned to remain functional, while showing increased environmental awareness. The cycle
is repeated until an objective decision can be made as to the environmental efficiency of the
The technique of life cycle analysis is a good way to examine the practicality of further
development of biopolymer materials. Only by exploring all implications of the product can its
true environmental responsiveness be judged. As society continues to become more aware of
environmental issues, the procedure of LCA will continue to be used more often. On the other
hand, further acceptance of integrated waste management techniques for biodegradable plastic
materials, involving efficient material use and disposal must also continue (Subramanian 2000).
ECONOMIC IMPACTS OF BIOPOLYMERS
From the viewpoint of industry, the greatest advantage of using biopolymers derived from
renewable feedstocks is their low cost. At a first glance, biopolymers appear to be a win-win
opportunity for the economy and the environment. However, as is the situation with
environmental issues, a closer look at the cost-performance ratio of biopolymers must be taken
in order to make sound economic decisions (Swift 1998).
According to Leaversuch (2002), cost is a stumbling block for synthetically derived
biodegradable plastic materials when they are directly compared with their conventional
counterparts. As the case with any new material, manufacturers must expect a minimum of two
years of losses before a profit is returned. Leaversuch also indicated that a key factor restricting
growth of biopolymer industries is that the infrastructure for sorting and composting organic
waste is developing more slowly than was initially expected.
Many reports paint a more optimistic picture for the economic promise of biopolymers. As
Salmoral et al. (2000) reported, a number of major chemical companies are gaining interest in
developing biopolymer technologies used to manufacture products from renewable resources.
Tharanathan (2003) reported that synthetic plastics will never be totally replaced by
biodegradable materials. However, he believes that in niche markets where the development is
feasible, there exists an opportunity for manufacturers to find a large profit.
One sector in which economic benefits exist from the use of biopolymer materials is in the
automotive industry. With respect to fiber reinforcements, widely employed traditional glass
fibres are abrasive, and quickly wear down processing equipment. The texture of flax fibres is
less coarse, prolonging the life of processing equipment (Stamboulis et al. 2000). Williams and
Pool (2000) identified that natural fibres are advantageous over synthetic ones because they
are less expensive and more readily available. The expansion of flax fiber incorporation into
automobile parts is a positive development for Canada’s agriculture industry, particularly in its
Another application of natural fiber reinforcement has been developed in the use of China reed
fiber to reinforce transport pallets. This was an economically sound decision, as the China reed
pallets are as mechanically stable as conventional pallets, but they are less expensive to create,
and need a shorter lifespan for cost recovery. Logistically, the China reed pallets are also more
economic than the conventional type because their lighter mass requires less fuel for transport
(Corbiere-Nicollier et al. 2001).
Work continues in the development of the biopolymer industry to a point where it is completely
economically competitive with the conventional plastic industry. Synthetic plastics are produced
on a large scale, while for the most part biopolymers are currently produced on a small scale.
The inexpensive nature of the renewable resource feedstocks is encouraging researchers and
industry officials to invest time to further develop these processes.
As the production of biopolymers expands, so too will the services associated with it. For
example, facilities where flax straw is decorticated and processed into fibers are necessary for
further expansion of flax fiber incorporation as material reinforcements (Lammers and Kromer
2002). In the case of microbially-grown polymers, large fermentation and separation facilities
are needed for the further use of such materials. As a general summary, it may be stated that
time will lead to greater economic strength for the incorporation of biopolymer materials into
THE FUTURE OUTLOOK FOR BIODEGRADABLE PLASTICS
There is room for growth and expansion in many areas of the biodegradable plastic industry.
Chau et al. (1999) estimates that plastic waste generation will grow by 15% per year for the next
decade. Carbon dioxide emissions from the formation and disposal of conventional plastics are
reaching epic levels. The complete substitution of petroleum-based feedstock plastics by
renewable resource-based feedstock ones would lead to a balanced carbon dioxide level in the
atmosphere (Dahlke et al. 1998). However, it is ludicrous to expect a full replacement of
conventional polymers by their biodegradable counterparts any time soon. Expansion into
particular niche markets seems to be the most viable option.
Researchers worldwide are interested in the area of biopolymer development. The German
government has stringent regulations in place regarding acceptable emission levels. In 1990,
the German government published a call for research and development of biodegradable
thermoplastics (Grigat et al. 1998). For this reason, many German material scientists and
engineers have focused their work on environmentally stable biodegradable plastics. Various
materials have been created by these researchers, including the Bayer BAK line which was
introduced in extrusion and injection moulding grades in 1996. Novamont, an Italian company,
introduced the Mater-Bi line for similar reasons. Queen Mary University in London, England has
a plastics department which is actively working on biocomposite development (Hogg 2001). As
a whole, all European nations are expected to follow the European Packaging directive, which
expects a material recovery of packaging waste. Organic recovery (composting spent
materials) is the most commonly applied waste reduction method (Schroeter 1998). European
nations are also expected to incorporate 15% w/w of recycled plastics into the manufacture of
packaging materials. Germany aims to better that level, as they set tier goal in 2001 for a 60%
incorporation of recycled plastics into new packaging materials (Fomin et al. 2001).
European nations are the front runners of biopolymer research, but impressive developmental
work has occurred, and continues to occur, in other geographical areas. The Chinese
government is responsible for a large population on a small land base. Therefore, the
preservation of space, and responsible disposal of waste are key considerations. For these
reasons, Chinese researchers are focussing on refinement of microbially produced PHA (Chau
et al. 1996). North American researchers, including those at the University of Saskatchewan,
are also interested in biopolymer development, as the agricultural industry will benefit from the
potential value added processing. The acceptance of the Kyoto Accord by the Government of
Canada is fueling a need for the reduction of use of fossil fuel feedstocks, and an increase in
the use of renewable resource feedstocks. Biodegradable plastics fulfill this requirement.
As the biopolymer industry grows, issues with production will be worked out. There are some
areas of concern that researchers are aware of, and are consequently focussing on. Multilayer
films containing starch and/or natural fibres tend to have adhesion problems (Frisoni et al. 2001,
Martin et al. 2001). The search for an ideal processing technique to circumvent this problem
continues. In this regard, Verhoogt and co-workers (1995) have concluded that additional
starch content in thermoplastic blends increases flexibility, but decreases mechanical strength.
As reported by Van Soest and Kortleve (1999), direct relations between processing, structure,
and properties of starch based materials are inconclusive.
Standards organizations such as the ASTM and ISO have published methods for material tests
on biodegradable plastic materials. A need for reviews and improvements of these tests has
come to light as industry expands its use of biopolymers. In particular, non-homogenities are
created in polymer materials by the clamps used for tensile tests (Nechwatal et al. 2003). The
nature of natural materials requires different considerations than those for synthetic materials.
The biopolymer industry has a positive future, driven mainly by the environmental
benefits of using renewable resource feedstock sources. The ultimate goal for those working in
development is to find a material with optimum technical performance, and full biodegradability.
There are a seemingly limitless number of areas where biodegradable polymer materials may
find use. The sectors of agriculture, automotives, medicine, and packaging all require
environmentally friendly polymers. Because the level of biodegradation may be tailored to
specific needs, each industry is able to create its own ideal material. The various modes of
biodegradation are also a key advantage of such materials, because disposal methods may be
tailored to industry specifications.
Environmental responsibility is constantly increasing in importance to both consumers and
industry. For those who produce biodegradable plastic materials, this is a key advantage.
Biopolymers limit carbon dioxide emissions during creation, and degrade to organic matter after
disposal. Although synthetic plastics are a more economically feasible choice than
biodegradable ones, an increased availability of biodegradable plastics will allow many
consumers to choose them on the basis of their environmentally responsible disposal.
The processes which hold the most promise for further development of biopolymer materials are
those which employ renewable resource feedstocks. Biodegradable plastics containing starch
and/or cellulose fibres appear to be the most likely to experience continual growth in usage.
Microbially grown plastics are scientifically sound, and a novel idea, but the infrastructure
needed to commercially expand their use is still costly, and inconvenient to develop.
Time is of the essence for biodegradable polymer development, as society’s current views on
environmental responsibility make this an ideal time for further growth of biopolymers.
The authors gratefully acknowledge the financial support for this project provided by the
Agriculture Development Fund (ADF) of SK Agriculture, Food, & Rural Revitalization, and the
University of Saskatchewan Summer Student Employment Program.
Aminabhavi, T.M., Balundgi, R.H., Cassidy, P.E. 1990. Review on biodegradable plastics.
Polymer Plastics Technology and Engineering. 29(3): 235-262.
Andreopoulos, A.G. 1994. Degradable plastics: A smart approach to various applications.
Journal of Elastomers and Plastics. 24(4): 308-326.
ASTM Standards, Vol. 08.01. 1998. D883-96: Standard Terminology Relating To Plastics.
New York, NY.: ASTM
Bastioli, C. 1998. Bak 1095 and Bak 2195: Completely biodegradable synthetic
Thermoplastics. 59(1-3): 263-272.
Bismarck, A., Aranberri-Askargorta, I., Springer, J., Lampke, T., Wielage, B., Samboulis, A.,
Shenderovick, I., Limbach, H. 2002. Surface characterization of flax, hemp, and
cellulose fibers; Surface properties and the water uptake behavior. Polymer
Composites. 23(5): 872-894.
Blanco, A. 2002. Just add water. Plastics Engineering. 58(10): 6
Bledzki, A.K., Gassan, J. 1999. Composites reinforced with cellulose based fibers. Progress In
Polymer Science. 24: 221-274.
Boustead, I. 1998. Plastics and the environment. Radiation and Physical Chemistry. 51(1):
Callister, W.D. 1999. Materials Science and Engineering: An Introduction. New York, N.Y.:
John Wiley and Sons.
Chandra, R., Rustgi, R. 1998. Biodegradable polymers. Progressive Polymer Science. 23:
Charron, N. 2001. Plastic Products and Industries. Statistics Canada Ref. No. 33-250-XIE.
Ottawa, Canada: Manufacturing, Construction, and Energy Division.
Chau, H., Yu, P. 1999. Production of biodegradable plastics from chemical wastewater – A
novel method to resolve excess activated sludge generates from industrial wastewater
treatment. Water Science and Technology. 39(10-11): 273-280.
Chiellini, E., Cinelli, P., Imam, S., Mao, L. 2001. Composite films based on biorelated agro-
industrial waste and PVA. Preparation and mechanical properties characterization.
Biomacromolecules. 2: 1029-1037.
Corbiere-Nicollier, T., Gfeller Laban, G., Lundquist, L., Letterier, Y., Manson, J., Jolliet, O.
2001. Life cycle assessment of biofibers replacing glass fibers as reinforcement in
plastics. Resources, Conservation, and Recycling. 33: 267-287.
Crawford, C. 2001. Developing Biobased Industries In Canada. Federal Biomass/Bioenergy
Strategy Framework (AAFC & NRCan).
Dahlke, B., Larbig, H., Scherzer, H., Poltrock, R. 1998. Natural fiber reinforced foams based on
renewable resources for automotive interior applications. Journal of Cellular Plastics.
Fomin, V.A. 2001. Biodegradable polymers, their present state and future prospects. Progress
In Rubber and Plastics Technology. 17(3): 186-204.
Fredrik-Selin, J. 2002. Lactic acid formed into biodegradable polymer. Advanced Materials
and Processes. 160(5): 13.
Frisoni, G., Baiardo, M., Scandola, M. 2001. Natural cellulose fibers: Heterogeneous
acetylation kinetics and biodegradation behavior. Biomacromolecules. 2: 476-482.
Grigat, E., Kock, R., Timmermann, R. 1998. Thermoplastic and biodegradable polymers of
cellulose. Polymer Degradation and Stability. 59(1-3): 223-226.
Guan, J., Hanna, M.A. 2002. Modification of macrostructure of starch acetate extruded with
natural fibers. ASAE Paper No. 026148. Chicago, Illinois. ASAE.
Hogg, P. 2001. Plastics, rubber, and composites at Queen Mary. Plastics, Rubber, and
Composites. 30(5): 193-194.
Hornsby, P., Hinrichsen, E., Tarverdi, K. 1997. Mechanical properties of polypropylene
composites reinforced with wheat and flax straw fibers. Journal of Materials Science.
Huang, J.C., Shetty, A.S., Wang, M.S. 1990. Biodegradable plastics: A review. Advances in
Polymer Technology. 10(1): 23-30.
Ichikawa, S. 1997. Fishhook. Canadian Patent No. 2198680.
Jopski, T. 1993. Biodegradable plastics. Starch. 83(10): 17-20.
Kokubo, T., Kim, H., Kawashita, M. 2003. Novel bioactive materials with different mechanical
properties. Biomaterials. 24: 2161-2175.
Lammers, P., Kromer, K. 2002. Competitive Natural Fiber Used in Composite Materials for
Automotive Parts. ASAE Paper No. 026167. Chicago, Illinois. ASAE.
Leaversuch, R. 2002. Biodegradable polyesters; Packaging goes green. Plastics Technology.
Ledward, D.A. 1998. Properties and applications of compostable starch-based materials.
Trends in Food Science and Technology. 41: 402-405.
Li, F.M., Guo, A.H., Wei, H. 1999. Effects of clear plastic film mulch on spring wheat yield.
Field Crops Research. 63: 79-86.
Lorcks, J. 1998. Properties and applications of mater-bi starch-based materials. Polymer
Degradation and Stability. 59(1-3): 245-249.
Martin, O., Schwach, E., Averous, L. Couturier, Y. 2001. Properties of biodegradable
multilayer films based on plasticized wheat starch. Starch. 53(8): 372-380.
Mukhopadhyay, P. 2002. Emerging trends in plastic technology. Plastics Engineering. 58(9):
Mulder, K.F. 1998. Sustainable production and consumption of plastics? Technological
Forecasting and Social Change. 58: 105-124.
Nakasaki, K., Ohtaki, A., Takano, H. 2000. Biodegradable plastic reduces ammonia emissions
during composting. Polymer Degradation and Stability. 70: 185-188.
Narayan, R., Pettigrew, C. 1999. ASTM standards help define and grow a new biodegradable
plastics industry. ASTM Standardization News. December: 36-42.
Nechwatal, A., Mieck, K., Reubmann, T. 2003. Developments in the characteristics of natural
fiber properties and in the use of natural fibers for composites. Composites Science and
Technology. 63: 1273-1279.
Orhan, Y., Buyukgungor, H. 2000. Enhancement of biodegradability of disposable polyethylene
in controlled biological soil. International Biodeterioration and Biodegradation. 45: 49-
Park, S.Y., Lee, B.I., Jung, S.T., Park, J.H. 2001. Biopolymer composite films based on k-
carrageenan and chitosan. Materials Research Bulletin. 36: 511-519.
Petkewich, R. 2003. Microbes manufacture plastic from food waste. Environmental Science
and Technology. 5: 175-176.
Sakiyama-Elbert, S., Hubbell, J. 2001. Functional biomaterials: Design of novel biomaterials.
Annual Review of Materials Research. 31: 183-201.
Sain, M. 2002. Process to Improve Thermal Properties of Natural Fiber Composites. Canadian
Patent No. 2350112.
Salmoral, E.M., Gonzalez, M.E., Mariscal, M.P. 2000. Biodegradable plastic made from bean
products. Industrial Crops and Products. 11: 217-225.
Schroeter, J. 1998. Creating a framework for the widespread use of biodegradable polymers.
Polymer Degradation and Stability. 59(1-3): 377-381.
Simon, J., Muller, H., Koch, R., Muller, V. 1998. Requirements for biodegradable water soluble
polymers. Polymer Degradation and Stability. 59(1-3): 107-115.
Stamboulis, A., Baille, C., Garkhail, S., Van Melick, H., Peijs, T. 2000. Environmental durability
of flax fibers and their composites based on polypropylene matrix. Applied Composite
Materials. 7(5-6): 273-294.
Stevens, E.S. 2003. What makes green plastics green? Biocycle. 44(3): 24-27.
Subramanian, P.M. 2000. Plastics recycling and waste management in the US. Resources,
Conservation, and Recycling. 28: 253-263.
Swift, G. 1998. Prerequisites for biodegradable plastic materials for acceptance in real life
composting plants and technical aspects. Polymer Degradation and Stability. 59(1-3):
Tharanathan, R.N. 2003. Biodegradable films and composite coatings: Past, present, and
future. Trends in Food Science and Technology. 14: 71-78.
Thurston, D., Lloyd, S., Wallace, J. 1994. Considering consumer preferences for
environmental protection in material selection. Materials & Design. 15(4): 203-209.
Van Soest, J., Kortleve, P. 1999. The influence of maltodextrins on the structure and properties
of compression molded starch plastic sheets. Journal of Applied Polymer Science.
Verhoogt, H., Truchon, F., Favis, B., St-Pierre, N., Ramsay, B. 1995. Morphology and
mechanical properties of blends containing thermoplastic starch and PHB. Annual
Technical Conference – ANTEC 95 (53rd). Boston, Mass.
Williams, G., Pool, R. 2000. Composites from natural fibers and soy oil resins. Applied
Composite Materials. 7(5-6): 421-432.